Alatabe, M. J.*
Environmental Engineering Department, Faculty of Engineering, University of Mustansiriyah, Baghdad, P.O. Box: 14022, Baghdad, Iraq.
Received: 09.01.2018 Accepted: 24.05.2018
ABSTRACT: The present study evaluates the suitability of activated carbon, prepared from Cane Papyrus, a plant that grows naturally and can be found quite easily, which serves as a biological sorbent for removal of Cu2+ ions from aqueous solutions. Fourier transform infra-red analysis for the activated carbon, prepared from Cane Papyrus confirms the presence of amino (–NH), carbonyl (–C=O), and hydroxyl (–OH) functional groups with Bath mode getting used to investigate the effects of the following parameters: adsorbent dosage (among the rates of 10, 20, and 30 g/L), pH values, Cu2+ initial concentration, and contact time. Results reveal higher efficiency (98%) of powdered adsorbent for removal of Cu2+ ions, which is found at pH=6 with 30 g/L activated carbon, prepared from Cane Papyrus, for a duration of 2 hours. The Freundlich isotherm model with linearized coefficient of 0.982 describes the adsorption process more suitably than the langmuir model, in which this rate equals to 0.899. Pseudo-second order kinetic equation best describes the kinetics of the reaction. Furthermore, it has been found that 0.5M HCl is a better desorbing agent than either 0.5 M NaOH or de-ionized water. The experimental data, obtained, demonstrate that the activated carbon prepared from Cane Papyrus can be used as a suitable adsorbent for Copper(II) ion removal from aqueous solutions.
Keywords: Natural Plants, Biosorbent, Activation, Removal Efficiency, Kinetics.
Heavy metal pollution has been one of the most challenging environmental problems due to its toxicity, persistence, and bioaccumulation tendencies (Delaila et al., 2008). Most industries produce and discharge metal-containing wastes mostly into water bodies, which affect the aesthetic quality of the water, while increasing the concentration of present metals (Donohue, 2004). Activities such as mining and smelting operations, wastewater treatment facilities, various agricultural works, and metal casting contribute significantly to the
Several techniques have been designed for removal of heavy metals from aqueous solutions, including ion exchange, chemical precipitation/co-precipitation, filtration, coagulation, membrane technologies, and commercial activated carbon (Inglezakis et al., 2004; Baccar et al., 2009). The major disadvantages of these methods lie in the cost involved, the efficiency of the processes, and disposal of wastes generated (Alatabe, 2012; Cheung et al., 2001). Technologies that treat Cu2+ contaminated waters include (i) adsorption both in batch and column operations (Moselhy et al., 2017; Hameed et al., 2007), (ii) coagulation, electro coagulation, and flocculation, (iii) ion exchange (Veli & Pekey, 2004), and (iv) membrane filtration (Bouhamed et al., 2016). Convenient design and operation has rendered adsorption in packed beds the most applicable practice among all these technologies, particularly within a frugal approach (Zhu et al., 2012). Adsorption processes are able to eliminate many contaminants in a multi-barrier approach. There is a growing interest in the application of plant biomass for water treatment in general and aqueous Cu2+ removal in particular (Futalan et al., 2011; Vernersson et al., 2002). The main advantage of plant biomass is that it is readily available and can work under almost-neutral pH (Lin & Wang, 2002). The contaminant removal mechanism by this class of material is not established. It is currently understood that the driving force for decontamination relies in its affinity with several species, present in the biomass structure (e.g. cellulosic groups of Ca2+, Mg2+, OH-, and –NH2,) (Prasad et al.,
2008). Relevant removal mechanisms include bio sorption, ion-exchange, and physical adsorption (Qin et al., 2006; Hanzlik et al., 2004). In recent years, several plant materials have been positively tested for Cu2+ removal such as (i) cinnamomum camphora (Chen et al., 2010)
and (ii ) modified barley straw (Pehlivan et al., 2012). The literature review indicates that Cane Papyrus is yet to be used for Cu+2 removal from industrial waste water. Therefore, this study presents the use of Cane Papyrus as a potential, novel, environmentally-friendly, and cheap adsorbent for elimination of Cu+2 ions from aqueous solution and wastewater samples. Usually industries seek out low cost methods for waste water treatment, hence they may option for low cost adsorbents. Although research reports show varieties of low cost adsorbents, all adsorbents are not available easily throughout the world (Alatabe, 2018).
The objective of the present study is to prepare activated carbon from can papyrus in order to increase the removal efficiency of the metals via adsorption, then to investigate the adsorption potential of activated carbon, prepared from Cane Papyrus in the removal of Cu+2 ions from aqueous solution, while investigating the effects of pH, adsorbent amount, contact time, and concentration of metal ions in the solution. The langmuir and Freundlich isotherms models are used to investigate equilibrium data. The adsorption mechanisms of Cu+2 ions onto activated carbon, prepared from Cane Papyrus, are also evaluated in terms of kinetics and thermodynamics.
MATERIALS AND METHODS
Fig. 1. Map of the marshes, south of Iraq
The dry biomass was ground to fine powder, using a hammer mill, and then weighed. After milling, the materials got dried in an oven at 105 °C for 24 h. To avoid further moisture absorption, samples were preserved in desiccators. Dried samples were then taken in a porcelain crucible and covered with lid to be placed in control muffle furnace at 750 °C for an hour. Afterwards, the carbonized cane papyrus samples got cooled and treated with alkali solution (sodium hydroxide) for its resultant leaching ash. After removal of ash from cane papyrus char, the char was washed and dried in oven. Two grams (2 g) of treated cane papyrus char was soaked in zinc chloride solution for 24 h (Cheung et al., 2001). Then the crucible was placed inside a muffled furnace so that it would
receive the required heat treatment. After activation with zinc chloride, the samples were washed with 1M hydrochloric acid solutions firstly and then with distilled water, until the pH value reached 7.0. After washing, the samples were dried in an oven at 105 °C for 24 h. Then the dried samples were preserved in desiccators to avoid further moisture absorption. The adsorbent showed a fluffy, highly porous, and rough microstructure, containing some voids and cracks which was suitable for the adsorption of Cu+2 ions. The concentration of Cu+2 ions in aqueous solution was analyzed, using Atomic Absorption Spectrometer (AAS). Mechanical shaker with adjustable speed time was used for agitation, while all pH rates were measured via a pH-meter.
One gram of activated carbon powder, prepared from can papyrus, was used for the adsorption of Cu+2 ions onto the surface of activated carbon, again prepared from Cane Papyrus via a mechanical shaker with the speed of 200 rpm at 25Co. The effect of adsorbent dosage was investigated by altering the initial mass of the adsorbent between 5 and 100 gm, with the optimum dosage used for subsequent processes. Similarly, depending on the pH, initial Cu2+ removal was initiated by contacting 0.0 to 5.0 g of the adsorbent with 100 ml Cu2+ solution for 5–l20 min in a closed cylindrical plastic vessel, 250 ml in volume.
Copper(II) Sulfate Pentahydrate (CuSO4.5H2O) was used as the source
of Cu2+ ion in a simulated effluent solution, made from water with a TDS (total dissolved solid) of 200 mg/L and a pH value of 7. Hydrochloric acid and sodium hydroxide solutions, both with a concentration of 1M, were used to adjust the pH value. In the prepared solution samples, the contaminant concentrations were 2.0, 3.0, and 4.5 mg/L. After equilibration for 60 min, the adsorbent was recovered. Residual Cu+2 ions on the surface of the used adsorbent was removed by getting washed three times with ultra-pure water. De-ionized water, 1M NaOH, and 1M HCl were tested as potential desorbing agents, wherein 40 ml of the agents was introduced into a l00 ml Teflon container, containing the recovered adsorbent, then to get equilibrated for 60 min at a speed of 200 rpm and T = 25Co. Following the equilibration, the aqueous solutions were centrifuged and the supernatant analyzed to determine the concentration of Cu+2 ions after desorption.
RESULTS AND DISCUSSION
Results from the Fourier transform infra-red showed a broad peak at 3000 1/cm with a high transmittance frequency, which can be attributed to either –OH or –NH groups. As shown in Figure 2.B, the band observed at
2550 1/cm is possibly due to C–H stretching vibrations of saturated aliphatic compounds, as reported by Smith, whereas the one at l750 1/cm can be attributed to –NH bending vibration of primary amines. A small peak was observed at l350 1/cm, corresponding to v(C–C) stretching vibrations of aromatic rings. The peaks, observed at l200 1/cmand l150 1/cm, corresponded to the C–O stretch of alcohols, carboxylic acids, esters, or ethers. The absorption band at 500 1/cm can be due to the presence of an alkyl halide. Also it was confirmed that mucilage extracted from Diceriocaryum species contained carboxyl functional group. The presence of acidic functional groups was responsible for its adsorptive trait. Furthermore, it was clearly stated from previous studies of natural plant materials that the biochemical characteristics of acidic functional groups were responsible for their metal ion uptake (Smith, 2011).
( A )
( C )
Table l. Chemical Composition of activated carbon, prepared from Cane Papyrus.
Compound Wt % Compound Wt %
l.l7 1.2 25.9 l.33 0.778 1.2 2.3
SrO BaO ll.7 2.7 1.1 17.6 2.0 l.24 1.5
Table 2. Characteristics of activated carbon, prepared from Cane Papyrus.
Physical Parameters Result
BET surface area (m2 /g) Micropore surface area (m2 /g)
Total pore volume (cm³/g) Micropore volume (cm³/g) Average pore diameter(Ao or l0−8 cm)
3.5 l.75 1.5 1.02 191
Surface area of the adsorbent was 3.5 m2 /g (Table 2). The average pore diameter of activated carbon, prepared from Cane Papyrus, ranged between l0 and 1000 × l0−8 cm, with the adsorbent classified as a meso-porous material. Similarly, reported BET surface areas of l.02 cm2/g and 3.75 m2/g for activated carbon from macadamia nuts were used for phenol removal and maize tassels for heavy metal removal from polluted waters, respectively, although adsorbents with higher surface areas have been widely reported in literature (Alatabe & Alaa, 2017).
The percentage of removing Cu+2 ions from aqueous solution was estimated by means of Equation (l):
100 Adsorption %
where Ci and Cf are the initial and final
metal ion concentrations, respectively.
Co Ce V
where qe is the amount of metal adsorbed in mg/g, with Ci and Ce representing initial
and equilibrium concentrations of metal ions in aqueous phase. V is the volume of the solution in liters (L) and W, the weight of the adsorbent used in grams.
Figure 3 demonstrates the effect of pH on the variation of adsorption on the time of contact at the experimental work conditions: 30g adsorbent dosage, volume =1L, and Cu2+ concentration= 5 mg/L. The initial pH of the solution was 8. Two other pH values of 6 and 2 were also investigated, with the best result achieved for the solution with pH value of 6. More alkaline solutions with pH values higher than 8 were not investigated, because metallic hydroxide (e.g. Cu(OH)2) could be
formed at high pH values in the alkaline range. Cu2+ ions was precipitated as Cu(OH)2, quite difficult to be segregated
Fig. 3. Impact of pH values on Cu2+ ions adsorption (%), using activated carbon, prepared from Cane Papyrus
All the curves correspond to 120 minutes, with Curve No.1, Curve No.2, and Curve No.3, representing 98%, 80%, and 60% of Cu2+ ion removal, respectively. The lines are not fitting functions; they simply connect points to facilitate visualization. Increase in Cu2+ ions removal along with the increase in pH values can be explained on the basis of a decrease in competition between proton and metal cat-ions for reactions with the same functional groups. Another parameter is the decrease in positive charge of the adsorbent, which results in a lower electrostatic repulsion between the metal cat-ions and the surface. Carboxyl and sulfate groups have been identified as the main sites for attachment of metal ions with the main chemicals in seaweed and, as these groups can have acidic property, their presence is pH-dependent. These groups generate a negatively-charged surface within pH range of 3.5-5.0. Moreover, electrostatic interactions among cationic species and this surface were responsible for metal uptake. As the pH rose, the ligands such as carboxylate groups in Sargassum sp. would be exposed, increasing the negative charge density on biomass surface, enhancing the attraction of metallic ions with positive charge and allowing the bio sorption onto the cell surface. By increasing pH, the rate of adsorption also rose, with the optimum pH of
6 for copper bio sorption. Copper ion forms an insoluble hydroxide, precipitated at pH values above 8, consequently leading to no adsorption. Obviously metal adsorption depends on the nature of the adsorbent surface. At low pH, the H+ ions compete with metal ions for the exchange sites in the system, thereby partially releasing metal ions.
Figure 4 shows, the increase of adsorption rate through raising the concentration of Cu2+ ions. A higher aqueous concentration of Cu2+ ions means more opportunities contact with a constant amount of the adsorbent.
Fig. 4. Effect of initial concentration of Cu+2 ions on the efficiency adsorption onto activated carbon, prepared from Cane Papyrus
Figure 5 demonstrates changes of aqueous Cu2+ ion concentrations as a function of time for an adsorbent mass loading of 30 g/L. It can be seen that Cu2+ ion removal increased very sharply at the beginning, reaching 60% after some 30 minutes. After 80 minutes, a plateau was reached at about 60% Cu2+ ion removal and maintained until the end of the experiment (120 minutes) at about 98%. Data from Figure 6 suggest that 2 hours (120 minutes) are a suitable duration to achieve a pseudo-equilibrium under the experimental
conditions of this work. Figure 5 summarizes the effect of adsorbent mass loading, varying from 10 g/L to 30 gm/L for Cu2+ ion removal within 2 hours. The efficiency of Cu2+ ion removal was 20%, 60%, and 98% for 10, 20, and 30 gm/L of activated carbon prepared from Cane Papyrus, with a volume of 1L and Cu+2 concentration of 5mg/L. This plateau at the end of curves was probably from saturation of the surface of adsorbent with metal ions, followed by adsorption and desorption processes that occur afterwards.
Fig. 6. Influence of various dosage of activated carbon, prepared from Cane Papyrus, on Cu+2 ion adsorption efficiency
Experimental data for the adsorbed metal against initial concentration were fitted into the langmuir and Freundlich adsorption isotherms. The langmuir model (Langmuir, 1916) assumes that the adsorption of an ideal gas on an ideal surface occurs only at fixed number of sites, with each site capable of only holding one adsorbent molecule (monolayer). It also assumes that all available sites are equivalent and there is no interaction between adsorbed molecules on adjacent sites. The linearized equation for langmiur model (Langmuir, 1918; Xiao & Thomas, 2004) is represented by Equation (3).
qe qmax bqmax Ce
l l l l
where Ce is the equilibrium concentration of the metal ion (mg/L); qe, the quantity of
Cu+2 ion adsorbed at equilibrium (mg/g); qmax, the maximum amount adsorbed
(mg/g); and b, the adsorption constant (L/mg). The plot of l/qe against l/Ce gave a
straight line with a regression coefficient of 0.8999 (Figure 7), indicating that the adsorption conformed to langmuir model. The maximum concentration of adsorbed Cu+2 ions as well as the adsorption capacity was calculated from the slope and intercept of the plot, which can be seen in Table 3. The conformity of the adsorption process to langmuir model was determined, using Equation (4):
where Rl is the separation factor; Co, the
initial metal concentration (mg/L); and b, the langmuir constant (l/mg). Rl > l, Rl = l,
0 < Rl < l, and Rl = 0 indicate unfavorable,
linear, favorable, and irreversible monolayer adsorption process, respectively. Results from this study had an Rl value between zero and one, indicating a
favorable adsorption process. This implies that chemisorptions process duly explain the adsorption of Cu+2 ions onto activated carbon, prepared from Cane Papyrus.
Table 3. Freundlich and Langmuir constants for Cu+2 ion adsorption onto activated carbon, prepared from Cane Papyrus
langmuir model Freundlich model
qmax(mg/g) b Rl(L/mg) R2 KF n R2
39.5 0.0315 0.0-1.0
Fig. 7. Langmuir plot for Cu+2 ion adsorption onto activated carbon, prepared from Cane Papyrus
The Freundlich isotherm mode (Freundlich, 1906) describes a multi-site adsorption for heterogeneous surfaces and can be represented by Equation (5);
q K Ce (5)
where Kf is the adsorption capacity (L/mg)
and l/n, the intensity of the adsorption, showing the heterogeneity of the adsorbent site as well as the distribution energy. Equation (6) was obtained by taking the logarithm of Equation (5):
e l e
logq log K logC (6)
A plot of logqe against logCe gave a linear graph with a regression coefficient
of 0.9823 (Figure 8), indicating that the adsorption also fits into Freundlich model. From the linearized coefficients, obtained from both models, the langmuir model described the adsorption process better than the Freundlich one. This suggests a chemisorptions rather than a physisorption process. Table 3 shows the constants, obtained for Freundlich and langmuir plot. A maximum adsorption capacity of 39.5 mg/g was obtained in this study for the adsorption of Cu+2 ions. The use of activated carbon, prepared from Cane Papyrus, is therefore a potential candidate for the removal of Cu+2 ions in water and wastewater.
Equations (7) and (8), respectively.
qe qt logqe (7)
2 2 t
qt K qe qe
where qe and qt stand for the amounts of
Cu+2 ions adsorbed at equilibrium and at the given time t, respectively, while kl and
Similarly, a linear graph (R2 = 0.983) was
obtained by plotting t/qt values against time
t (Figure 9). The pseudo second-order best described the kinetics of the adsorption process, which agreed with other results, reported in the literature. Results, obtained from the kinetic plot, favors chemisorptions mechanistic pathway rather than physisorption.
Fig. 9. Pseudo second-order kinetics for Cu+2 ion adsorption onto activated carbon, prepared from Cane Papyrus
Mechanism-Based Model Weber-Morris in Equation 9 was used to ascertain whether intra-particle diffusion or film diffusion (external diffusion) is the rate-controlling step.
qtKd t I (9)
where kd is the intra-particle diffusion rate
constant (mg/g min−0.5) and I (mg/g), a constant describing the thickness of the boundary layer. A linear plot of qt versus t1/2 passing through the origin suggests
intra-particle diffusion as the sole rate-determining step; however, if a linear plot was obtained, which did not pass through the origin, it meant the adsorption process was controlled by more than one mechanism. In this study, a linear plot was obtained that did not pass through the origin (Figure 11), suggesting that the mechanism of the reaction is multi-linear and the rate-limiting reaction was controlled both through film diffusion and intra-particle diffusion.
Fig. 11. Intra-particle diffusion model plot for Cu+2 ion adsorption onto activated carbon, prepared from Cane Papyrus
This study was carried out to assess the most suitable desorbing agent for eluting adsorbed Cu+2 ions from the surface of activated carbon, prepared from Cane Papyrus. The effects of de-ionized water, 0.5M NaOH, and 0.5M HClsolutions were tested for their ability to remove the adsorbed Cu+2 ions from the surface of the adsorbent. HCl was a better desorbing agent, capable of recovering 60% of Cu+2 ions, adsorbed to the surface of the adsorbent. NaOH and de-ionized water showed desorption efficiencies of 30% and 2%, respectively. Desorption is beneficial for the separation and enrichment of Cu+2 ions as well as the regeneration of the adsorbent.
The adsorption ability of powdered activated carbon, prepared from Cane Papyrus, was investigated and found
effective for the removal of Cu+2 ionsfrom wastewater. Acidic functional groups, present on the surface, and sustainability of the adsorbent are believed to be responsible for the removal of Cu+2 ions from aqueous media. The Freundlich isotherm model gave a better description of the adsorption process than the langmuir isotherm model. Pseudo-second order kinetics best described the kinetics of the reaction, while 0.5 M HCl was a better desorbing agent than 0.5 M NaOH as well as de-ionized water.
Journal of Scientific Research in Science, Engineering and Technology, 3(6): 2394-4099. Alatabe, M.J. (2018). A Novel Approach for Adsorption of Copper (II) Ions from Wastewater Using Cane Papyrus. International Journal of Integrated Engineering. 10(1): 96-102.
Baccar, R., Bouzid, J., Feki, M. and Montiel, A. (2009). Preparation of activated carbon from Tunisian olive-waste cakes and its application for adsorption of heavy metal ions. J. Hazard Mater, 162(2-3): 1522–1529.
Bouhamed, F., Elouear, Z., Ouddane, B. and Bouzid, J. (2016). Multi-component adsorption of copper, nickel and zinc from aqueous solutions onto activated carbon prepared from date stone. Environmental Science and Pollution Research, 23(16): 15801–15806.
Cheung, C.W., Porter, J. F. and McKay, G. (2001). Sorption kinetic analysis for the removal of cadmium ions from effluents using bone char. Water Research, 35(3): 605-621.
Chen, H., Dai, G., Zhao, J., Zhong, A., Wu, J. and Yan, H. (2010). Removal of copper(II) ions by a biosorbent —Cinnamomum camphora leaves powder. J. Hazard Mater, 177(1-3): 228–236. Delaila, T.N., Luqman, C.A., Zawani, Z. and Abdul, R.S. (2008). Adsorption of copper from aqueous solution by Elais Guineesis kernel activated carbon. J. Eng. Sci. Technol. 3: 180–189. Donohue, J. (2004). Copper in Drinking-water, World Health Organization.
Dorris, K. L., Zhang, Y., Shukla, S.S., Yu, B. and Shukla, A. (2000). The removal of heavy metal from aqueous solution by sawdust adsorption removal of copper. J. hazard mater, 80(1-3): 33- 42.
Freundlich (1906), HMF Over the adsorption in solution. J. Phys. Chem., 57(3): 85–471.
Futalan, C.M., Kan, C.C., Dalida, M.L., Hsien, K.J., Pascua, C. and Wan, M.W. (2011). Comparative and competitive adsorption of copper, lead, and nickel using chitosan immobilized on entonite. Carbohydr Polym, 83(2): 528–536.
Hanzlik, J., Jehlicka, J., Sebek, O., Weishauptova, Z. and Machovic, V. (2004). Multi-component adsorption of Ag(I), Cd(II) and Cu(II) by natural carbonaceous materials. Water Res., 38(8): 2178– 2184.
Ho, Y.S. and Mckay, G. (1999). Competitive sorption of copper and nickel ions from aqueous solution using peat. Journal of the International Adsorption Society. Adsorption, 5(4): 409–417. Inglezakis, V. J., Loizidou, M. M. and Grigoropoulou, H. P. (2004). Ion Exchange Studies on Natural and Modified Zeolites and the Concept of Exchange Site Accessibility. Journal of Colloid and Interface Science, 275 (2): 570-576.
Langmuir, I. (1916).The constitution and fundamental properties of solids and liquids. J. Am. Chem. Soc.,38(11): 2221–2295.
Langmuir, I. (1918). The adsorption of gases on plane surfaces of glass, mica and platinum. J. Am. Chem. Soc.,40(9): 1361-1403.
Lin, S. H. and Wang, C. S.(2002). Treatment of high-strength phenolic wastewater by a new two-step method. Journal of Hazardous Materials, 90(2): 205-216.
Mukesh, P. and Thakur, L.S.(2013). Heavy Metal Cu, Ni and Zn: Toxicity, Health Hazards and their removal techniques by Low Cost Adsorbents: A Short Overview. International Journal of Plant, Animal and Environmental Sciences, 3(3): 143- 157.
Moselhy, K.M., Azzem, M.A. , Amer, A. and. Al– Prol, A.E.(2017). Adsorption of Cu(II) and Cd(II) from Aqueous Solution by Using Rice Husk. Adsorbent. Phys. Chem. Ind. J.,12(2): 109-122. Patil, K.P., Patil, V.S., Nilesh, P. and Motiraya, V. (2012) . Adsorption of Copper (Cu2+) & Zinc (Zn2+) Metal Ion from Wastewater by Using Soybean Hulls and Sugarcane Bagasse as Adsorbent. International Journal of Scientific Research and Reviews, 1(2): 13-23.
Pollution is licensed under a" Creative Commons Attribution 4.0 International (CC-BY 4.0)" Prasad, M., Xu H.Y. and Saxena, S. (2008).
Multi-component sorption of Pb(II), Cu(II) and Zn(II) onto low-cost mineral adsorbent. J. Hazard Mater, 154(1-3): 221–229.
Qin, F., Wen, B., Shan, X.Q., Xie, Y.N., Liu, T., Zhang, S.Z. and Khan, S.U. (2006). Mechanisms of competitive adsorption of Pb , Cu, and Cd on peat. Environ Pollut., 144(2): 669–680.
Smith, B.C.(2011). Fundamentals of Fourier Transform Infrared Spectroscopy, Second Edition, Taylor and Francis Group.
Veli, S. and Pekey, B. (2004) Removal of copper from aqueous solution by ion exchange resins. Fresen. Environ. Bull., 13(3b): 244–250.
Vernersson, T., Bonelli, P.R., Cerrela, E.G. and Cukierman, A.L. (2002). Arundo donax cane as a precursor for activated carbons preparation by phosphoric acid activation. Bioresour. Technol., 83(2): 95–104.
Xiao, B. and Thomas, K.M. (2004). Competitive adsorption of aqueous metal ions on an oxidized nanoporous activated carbon. Langmuir, 20(11):4566–4578.